Mix-Solvothermal Syntheses, Characterization, and Properties of New Zinc Diphosphonates with Zn−O−P Chains, Layers, and 3D Frameworks
Fu, Ruibiao; Hu, Shengmin; Wu, Xintao; Crystal Growth & Design 7 (2007) 1134–; doi:10.1021/cg060833m

data_4504128
_publ_section_title
;
 Mix-Solvothermal Syntheses, Characterization, and Properties of New Zinc
 Diphosphonates with Zn&#x2212;O&#x2212;P Chains, Layers, and 3D
 Frameworks
;
_journal_issue                   6
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              1134
_journal_paper_doi               10.1021/cg060833m
_journal_volume                  7
_journal_year                    2007
_chemical_formula_sum            'C4 H13 N O6 P2 Zn'
_chemical_formula_weight         298.46
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                92.918(4)
_cell_angle_beta                 98.418(6)
_cell_angle_gamma                90.801(6)
_cell_formula_units_Z            2
_cell_length_a                   4.8852(18)
_cell_length_b                   9.986(4)
_cell_length_c                   10.432(4)
_cell_measurement_reflns_used    1386
_cell_measurement_temperature    130.15
_cell_measurement_theta_max      27.4835
_cell_measurement_theta_min      3.9566
_cell_volume                     502.7(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      130.15
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.981
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0137
_diffrn_reflns_av_sigmaI/netI    0.0236
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            3851
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         3.95
_exptl_absorpt_coefficient_mu    2.765
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.7324
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.972
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             304
_exptl_crystal_size_max          0.6000
_exptl_crystal_size_mid          0.1000
_exptl_crystal_size_min          0.0800
_refine_diff_density_max         0.438
_refine_diff_density_min         -0.513
_refine_diff_density_rms         0.081
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.112
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     179
_refine_ls_number_reflns         2270
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.112
_refine_ls_R_factor_all          0.0244
_refine_ls_R_factor_gt           0.0218
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0259P)^2^+0.4136P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0556
_refine_ls_wR_factor_ref         0.0575
_reflns_number_gt                2111
_reflns_number_total             2270
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg060833mrom20061123_040212.cif
_cod_data_source_block           8
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        502.6(3)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4504128